Copper (ii) adsorption by calcium alginate shea butter cake
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201320Copper (II) Adsorption by Calcium-alginate Shea Butter CakeMuibat Diekola Yahya (Corresponding author)Department of Chemical Engineering, Federal University of Technology, Minna,P.M.B. 65, Nigeria. E-mail: firstname.lastname@example.orgI.A. Mohammed-Dabo, A.S.Ahmed, A.S. OlawaleDepartment of Chemical Engineering, Ahmadu Bello University, Zaria,P.M.B. 810261, Nigeria.AbstractThis study investigated the utilization of modified shea butter cake for the removal of Cu(II) ions from aqueoussolution. Instrumental analysis such as Fourier transform infrared spectroscopy (FT-IR), Scanning electronmicroscopy (SEM), X-ray Diffractometer (XRD) was used for the characterisation of the solid sorbent. Batchequilibrium study was carried out to evaluate the adsorption capacity, and process parameters such as initial metalion concentration, time, pH, and adsorbent dosage. An optimum pH of 5, equilibrium time of 30mins and adsorbentdosage of 40 beads was obtained. The Langmuir and Freundlich isotherms were used to fit the experimental data andvalues fits the Langmuir more adequately with correlation coefficient unity (1.000) at 10mg/l of initial metal ionconcentration. The Kinetic study using the Pseudo-first-order and pseudo-second were used to determine the rateconstants and experiments data best fits the pseudo-second –order with calculated amount adsorbed approximatelyequal to the experimental values. The results indicate that modified shea butter cake could be employed as anadsorbent for the removal of copper (II) ions in an aqueous solution.Keywords: Shea butter cake, process parameters, kinetics, Copper (II),
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201321IntroductionThe activities of man through the growing and development of the small and medium scale enterprise has graduallykept on the increaseof copper (II) ions discharge into the environment. Thousands of years ago, the use of copperwas limited to making tools and other utensils, but now, it is widely used in electrical wire, coins, ornamentalobjects, jewellery, pharmaceuticals, fungicides (Odukoya and Ajayi, 1987; Wu et al., 1999) and mining activities(Hansen et al., 2010). These consequently have impact on the threshold limit.Copper toxicity can occur in plantsgrowing in polluted soils, and animals grazing on these plants, through the food chain. In humans about 10-20mg oforally ingested Cu may cause intestinal discomfort, dizziness and headaches, while ingestion of Cu salts in excess of500-100mg have caused fatal acute poisoning such as vomiting, diarrhoea with bleeding, circulatory collapse, failureof the liver and kidneys and severe haemolysis (Johnson, 1997). The maximum permissible limit of copper indrinking water is 2mg/L (Larous et al., 2005). A wide variety of treatment technologies for the decontamination ofthis metal-polluted effluent have been investigated and developed. These are chemical precipitation, ion exchange,adsorption, solvent extraction, membrane processes and electrochemical techniques. Adsorption process via the useof agricultural waste material is however been recently utilised because it is readily available, it has low energyconsumption, eco-friendly, and cost effective.The use of the Shea Butter Cake is proposed for the adsorption of copper in this study. Shea butter cake is the residueobtained after the extraction of the butter from the shea butter seed. Nigeria is blessed with the Shea butter tree withan estimated production output of 250,000 metric tonnes per annum (Peter, 2004). Although this has not beenoptimally utilised, cottage industry are gradually indulging in the shea butter production which obviously will lead tothe increase in the cake production. Studies have shown that the presence of the cake into the environment causesnuisance as they are non-bio-degradable and are un-palatable to livestock (He et al., 2007; Nitiema, 2010).Limitedwork has been reported in the utilisation of shea butter cake for adsorption processes.Yahya et al., (2012) used thecake in the raw and modified form for the removal of Pb (II) ions in an aqueous solution. It is however proposed touse theshea butter cake by modifying it with calcium alginate for the adsorption of copper (II) ions in aqueoussolution so as to serve the double benefit of treating a waste polluted water streams and revenue generation to theproducing industry. It will also provide a baseline of information and data for further research.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 2013222. Materials and MethodsThe shea butter fruits were collected from the farmland of Sabon-Dagaward inMinna, Niger state, Nigeria. Thecollected biomaterials were thoroughly washed with tap water to remove soil and dusts, and then further washed withdistilled water and dried in an oven at 80oC until a constant weight is achieved (Önate, 2009).The dried seed isgrinded to smoothness with a blender (Moulinex) and sieved using an electrical sieve shaker (Endecotts England BS410/1986) to obtain a powder <250µm particle size. Some physical processes such as churning andmixing was done.Warm water was used to press out the oil and over-float thefats. The fat was skimmed and heated to evaporate theexcess water molecules. The oil was decanted and filtering was done. The residue obtained after filtrationis the SheaButter Cake. This is air-dried until a constant weight is obtained and stored in a polyethene bag for further use.2.1 Preparation of shea butter cakeThe Modified shea butter cake MSBC) was prepared by dissolving 1g of sodium alginate (1% w/v) into 100ml ofdistilled water at a temperature of 65oC on a constant temperature magnetic stirrer(LabTech 78HW-1) (Fiol et al.,2006). The gel was completely dissolved and allowed to cool down at room temperature (25oC) and thereafter 2g ofshea butter cake (<250 µm) was added. An intense agitation was maintained on the magnetic stirrer in order toproduce homogeneous mixture of alginate and the powder. Afterwards the solution was added drop wise via ahypoject IV 110108syringe to a solution of 0.1M calcium chloride dihydate (CaCl2.2H2O) under soft agitation. TheCalcium atoms from the CaCl2 will cross link to form salt bridges between the α-L-guloronic acids (G) blocks of thesodium alginate (Onate, 2009). As a result of this, the alginate chains wrapped up the sorbents to form beads(Khorramabadi et al., 2011). The entrapped shea butter cake in the calcium alginate (CA) beads were cured in theCaCl2 solution for 24hr. Hard spherical beads of similar sizes containing 2% (w/v) of shea butter cake now calledmodified shea butter cake (MSBC) were filtered and rinsed several times with distilled water to remove excess Ca2+ions. The obtained beads were covered with abundant distilled water and stored in the fridge at around 4oC forfurther use.2.2 Preparation of metal solutionsDeionized water obtained from deionizer was used to prepare all solutions. All glass wares were soaked in 5% nitricacid for 24hr and repeatedly washed with doubly distilled deionized water followed by drying at 353K for 5 hr. so as
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201323to avoid contamination. Stock solution (1000mg/L) of copper was prepared by dissolving 2.6847g of analytical gradecopper chloride dihydrate (CuCl2.2H2O) in 100ml of deionized water and dilute to1 litre in a volumetric flask withdeionized water.2.3 Characterisation of adsorbentThe shea butter cake was characterized using the Fourier Transform-Infrared Spectrophotometer (FT-IR-8400S,Schimadzu Japan) in order to determine the functional group. The sample was prepared using KBr discs and thespectral range was varied from 4000cm-1to 400cm-1. The surface morphology of the sorbents was also studied withHigh Resolution Scanning Electron Microscope (EVO MA 10 Carl Zeiss). The X-ray diffraction (XRD) analysis wascarried out to determine the mineral composition, and crystalinity of the cake.2.4 Batch Equilibrium studyExperiments were carried out in batch mode using series of 250ml conical flasks with cork. 50ml of metal solution invarious concentrations ranging from 4mg/l, 6mg/l, 10mg/l, 50mg/l, 100mg/l, and 200mg/l were added to 40 beads ofthe modified shea butter cake on Stuart Scientific flask shaker at a speed of 200rpm. Agitation was carried out forover 360 minutes to ensure equilibrium although no significant change was recorded after 120 minutes as saturationhad been reached. All other parameters studied were therefore fixed at 120 minutes. After agitation, the beads werefiltered using Whatman filter paper (110cm) and metal concentration in the liquid phase was analysed using FlameAtomic Absorption Spectrophotometer Varian SpectrAA 220FS.The metal concentration in the the solid phase qe (mg.bead-1) was calculated from the difference between the initial,Ci and equilibrium, final, Ce metal concentration in solution (mg.L-1). The uptake of the sorbent was calculatedaccording to the next equation:( )NVCeCiqe −= (1)Where V(L) is the solution volume and N is the amount of beadsTo compute the sorption percentage, %R
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201324100% ×−=CiCeCiR (2)2.5 Kinetic study on Cu (II) adsorptionSorption kinetics was studied for initial concentrations of Cu ranging from 4mg/l-to 200mg/l. Metal solutions wereprepared by serial dilution and pH of 5 was maintained throughout. For each contact time, content of the flasks wasfiltered and copper concentration in solution was analysed. The studied time range was fixed at120minutes.2.6 Initial pH effect on Cu (II) adsorptionEffect of initial pH on Cu (II) sorption onto modified Shea butter cake was studied in order to obtain information onthe role of H+in Cu(II) uptake.pH values was from 1to 10 and initial metal concentration was around 250mg/l. ThepH of the adsorbate solution was adjusted with either 1 M NaOH or 0.1 M HCl without increasing the initialvolume of the solution significantly. Contact time was 120minutes.2.7 Effect of Adsorbent DosageAdsorbent dosage was varied from 40 beads-240 beads in 50ml of Copper (II) solution at a concentration of250mg/L. This was agitated for 120minutes at a speed of 200rpm. Solutions were filtered and residual metalconcentrations was analysed as statedpreviously.3. Discussions of results3.1 Characterisation of adsorbent materialThe IR spectra (Fig. 1) indicate that the RSBC possess different surface structure. There are some Absorption above3000/cm which suggests that it is unsaturated (contains C=C).Absorption is at the low end of the range (i.ebelow1700/cm) this suggest that the compound is probably amide or carboxylate. Additional moderate band in therange 1200-1000 and 800-600 implies simple hydroxyl compound. The shifting of the band of the O-H (Phenol)at1374.33/cm to 1440.87 of the loaded sample is attributed to O-H (phenol) bonding. Complete disappearance of thealiphatic nitro-compounds from the loaded sample also indicated adsorption of the metal at 1522.85/cm. A shift inthe peak at 1615 to 1633.76 of the loaded sorbent can be attributed to the stretching of C=O corresponding tocarbonyls, olefinic C=C stretching frequencies of hemicelluloses, lignin and amino groups. This was more prominentin the loaded sorbent indicating higher sorption due to structural modification (Akhtar et al., 2010). The sharp peak
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201325observed at 1741.78forsheabuttercake is assigned to C-O bond of carboxylic or its ester and itscompletedisappearance on the Cu-loaded sorbent inferred that the copper metal bonded to the shea butter cakethrough interaction with active groups OH, COOH (Minamisawa et al.,2004).Emerging of new bands on themodified sorbents at 3154.68; 3458.48; 3777.71 may be attributed to binding of –OH group with the polymericstructure.Fig. 2 shows the XRD patterns of Shea Butter Cake. The non-appearance of major peaks indicated that the sorbent isamorphous in nature. A very weak peak was observed at 26o2Θ diffraction anglewhich was attributed to quartzstructure of the silica (Kumagai et al., 2010)that may have been introduce during air-drying .Fig.3: depicts the SEM image of the Shea butter cake at 1KX and 3KX magnification. The micrographs indicatedthat the surface was irregular and porous in nature. The micrographs also depict the presence of superficial layers ofprotective silica and some natural resin.3.2 Effect of Time and initial metal ion concentrationFig. 4 shows the effect of Time and initial metal ion concentration;there was a sharp increase in percentage removalof the metal ions from the starting initial concentration value to the next level before saturation is reached. At lowerinitial concentration almost all the sites are filled during adsorption as there is a greater interaction between the metalion and sorptive sites but as the concentration increases more Cu(II) are left unadsorbed due to saturation of theadsorptive sites . This high initial rate of adsorption is as a result of increase in concentration which provides thedriving force that helps to overcome mass transfer resistance between the metal ion and adsorbent (Ibrahim et al.,2010).The amount of copper (II) ions adsorbed at equilibrium increases from 0.094mg/g to 4.64 mg/g as the initialmetal ion concentration was increased from 4 to 200 ppm.In relation to time, the rate of metal ion removal is found to be very rapid during the first 30 minutes of adsorption,thereafter, it is almost constant and then gradually decreases at higher concentrations. No significant change in metalion removal is observed after 120 minutes. Basically for the lower concentration metal ion solution, the maximumpercentage removal was achieved within 30minutes while for the higher concentration metal solution it was after1hour of agitation time. The rate of percentage metal removal is higher at the beginning firstly because of the affinity
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201326the sorbates has for the sorbent. Secondly, it may be due to the modification with calcium alginate. This played animportant role in the rigidity, enhanced porousity of the sorptive sites, resistance to leaching of the organiccomponent into the solution. This is justified in this study as percentage removal increased to over 90% asconcentration builds as high as 250mg/L. Authors that have used calcium alginate successfully for adsorptionprocesses to mention a few are Fiolet al., (2003); Khorambadiet al., (2011).3.3 Effect of pHThe pH governs the speciation of the metals in aqueous solution and also affects the dissociation of active functionalsites on the sorbent (Kazemipouret al., 2008). Notably is this as shown in Fig. 5. The percentage removal of Cu usingshea butter cake increases progressively from 1.4% at pH of 2 to 92.3%% at pH value of 5. This then gradually dropsat pH of 6 and remain almost constant up to pH of 10. At lower pH values (pH 2) biosorption was low as a results ofprotons (H+or H30+) domination to compete with the cations in the aqueous solution to occupy the shea butter cakesurface. Increasing the pH from 3 to 5 bring about a progressive increase in the biosorption which is as a result ofdecrease in the protons and consequently lowering the electrostatic repulsion between the Cu(II) and surface sites.The maximum percentage removal occurred at pH of 5 which agrees quite well with the work of Benaissa andEloudchi (2011) in their study of Cu(II) from aqueous solution using activated sludge. Beyond pH of 5, insolublecopper hydroxides starts precipitating resulting in lower amount of Cu(II) sorbed at equilibrium (Villaesusa et al.,2004).3.4 Effect of Adsorbent DosageFigure 6 shows the adsorption of Cu(II) with modified shea butter cake at varying adsorbent dosage (40beads-200beads), 250mg/L of initial metal concentrationand agitation speed of 200rpm at 120mins.Amount adsorbed of themetal ions decreases with increase in adsorbent dose. For example,the amount adsorbed at 40 beads is0.2525mg/bead this then reduces drastically to 0.070mg/beads at 200beads of the adsorbent mass. This reduction isas a result of using large amount of adsorbent dose which leaves the active sites partially filled and some sites evenvacant. This was justified by the work of Hansen et al., (2010) who reported that the larger the amount of solidbiomass, the lower the equilibrium concentration; Khan et al., (2011) further affirmed this in his study that increasing
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201327the biosorbent dosage may lead to some of the sites unsaturated and consequently decrease in biosorption capacity.The decrease in amount adsorbed may be further explained by the fact that aggregation of adsorbent particle doesoccur as adsorbent dosage is increased and this results to longer diffusion path length (Zheng et al, 2009).The reverseis the case with percentage removal of the metal ions from the solution. It rather, increases with increase inbiosorbent mass due to larger surface area on the sorbent and thus creates easy penetration of the metal ions to theadsorption sites (Ibrahim et al., 2010).3.5 Adsorption KineticsIn order to investigate the adsorption of Cu(II) on modified shea butter cake (MSBC), adsorption kinetic study usingthe pseudo-first –order (Lagergren, 1898) and pseudo-second-order, kinetic models (Ho and Mckay, 1999) were usedto predict the rate constants. These rate controls the residence time and the mechanism involved in the adsorbateuptake in the solid - solution interphase (Naiyaet al., 2009). The conformity between the calculated amount adsorbedand experimental data is determined by correlation coefficient (R2).3.5.1 Pseudo-first –order-modelThe pseudo first-order equation of Lagergren is generally expressed as follows:( ) ( ) tKqqq ete303.2loglog 1−=− (3)Where qe is the amount of adsorption capacity at equilibrium (mg/g), qt is amount adsorbed at time t, K1 is thepseudo-first-order rate constant (min-1).The values of qe and K1 for the pseudo-first-order kinetic model were determined from the intercepts and the slopesof the plots of log (qe-qt) versus time, respectively. The values are given in Table 1.From the linear regressionequation, the correlation coefficient R2was 0.5496 at 4mg/L and 0.4333 at 6mg/l. These were quite low and are notshown on the plot except for the non-linear regressions that were above 60% in correlation co-efficient. There is awide variation between the calculated and experimental values. This shows that the adsorption does not follow thefirst order which follow similar observation of other authors (Hansen et al., 2010; Kosasih et al., 2010; Gündoĝan etal., 2004).
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 2013283.5.2 The pseudo-second-order model : This can be expressed as:( )22 qtqeKdtdqt−= (4)Where K2 is the pseudo-second–order rate constant (g/mg min). Integrating with boundary conditions, qt=0 at t=0and qt=qt at t=t, results in the following equation:tqeqeKqtt1122+= (5)The initial sorption rate, h(mg/mg min), at 0→t can be defined as22qeKh = (6)Re arranging and substituting Eq (6) into Eq (5) givestqehtqt+=11(7)The value of qe is determined from the slope of the plot ofqttversus t (Fig. 9), and h isobtained from theintercept. The values of qe, K2, h and R2are shown in Table 2. The graph is linear for second-order than that of thefirst- order model. The experimental values (qe,exp.) correlated well with the calculated (qe,calc.) values for pseudo-second –order model than the pseudo-first-order, the correlation coefficient R2is closer to unity at 4mg/L, 6 mg/l50mg/l, 100mg/l and exactly 1.00 at 10mg/l . The initial sorption rate h can also be seen to be quite adequate fromTable 2 indicating a very fast sorption rate .Therefore the adsorption can be said to follow pseudo-second-order-model adequately which were well justified by the work of Zhang et al 2011; Gündoĝan et al., 2004).
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 2013293.6 Adsorption Equilibrium IsothermEquilibrium data were analysed using the Langmuir and Freundlich isotherm to understand the Cu(II) ions-modifiedshea butter interaction.eLLLeeCKaKqC+=1(8)eFe CnKq log1loglog += (9)Eq.(8) and (9) are Langmuir and Freundlich equations. In these equations, Ce and qe are the equilibriumconcentrations in the solution (mg/l) and on the modified shea butter cake (mg/g) respectively: aL (l/mg) and KL(l/g)are the Langmuir constants for the Cu(II) ions-modified equilibrium and monolayer capacity. KF (l/g) is Freundlichconstant and 1/n is heterogeneity factor.From Table 3, parameters obtained after correlation of experimental data to Langmuir and Freundlich showed goodcorrelation coefficient with the best fits for Langmuir model. Li et al., (2004) reported that the Gibbs free energy canbe calculated according to the equation ΔG= -RTln KL and the results shows that at higher Langmuir constant the ΔGwas smaller and invariably a higher spontaneity of the adsorption process. At KL310.00 L/g, the ΔG was -14.308 andcorrelation coefficient R2was exactly 1.0000. The dimensionless equilibrium parameter or the separation factorRL(Panda et al., 2007) was also calculated from the Langmuir equation from the expression:RL=iLCK+11(10)Where Ci and is the initial concentration of the Cu(II) ion and KLis the Langmuir constant. If adsorption isfavourable, Then RL must be within 0 to 1, while RL>1, RL=1 and RL = 0, respectively describe unfavourable, linearand irreversible adsorption. Here the RL value is within 0 to 1 and this indicates that the adsorption of Cu ions is wellfavoured on the modified shea butter cake.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201330Freundlich model did not provide as good determination coefficients as the Langmuir model. However, Freundlichmodel was used to calculate KF and1/n which are the parameters associated to the adsorption capacity and adsorptionintensity respectively The higher the 1/n, the higher will be the affinity and heterogeneityof the adsorbent sites.Thevalues of 1/n as shown on Table 3 was less than 1 and thus indicate that the adsorption was beneficial (Manet et al.,2007; Naiya et al., 2009).4. ConclusionsShea butter cake entrapped in calcium alginate effectively removes copper (II) ions from aqueous solution. Hydrogenion (H+) plays an important role on the effect of pH and an optimum pH of 5 was obtained for adsorption of theCu(II) before precipitation of the hydroxides. The FT-IR analysis indicate the main active groups such ascarboxylates, hydroxyl and the phenols as being responsible for the sorption. The Kinetic isotherm of Pseudo-second-order best fits the experimental and correlation coefficient of exactly 1 obtained at 10mg/l of initial metal ionconcentration. A very high amount adsorbed (qmax) of 161.290mg/g was achieved on subjecting experimental data tothe Langmuir equilibrium isotherm which suggest monolayer adsorption, this almost double that obtained for theFreundlich Isotherm. However, on comparison with other agricultural waste (Table 4) for Cu (II) adsorption, the qmaxwas on the high side for both Langmuir and Freundlich isotherms. The entrapment of the Shea butter cake in thecalcium alginate gel gave an improvement in the sorption capacity.The thermodynamic property ΔG indicate thespontaneity of the process and reaction is an exothermic one.ReferencesAkhtar, M.,Iqbal, S.,Kausar, A.,Bhanger, M.I.,Shaheen, M.A.(2010). An economically viable method for theremoval of selected divalent metal ions from aqueous solutions using activated rice husk. Colloids andSurfaces B: Biointerfaces75 149–155Alloway, B. J. and Ayres. D.C. (1997). Chemical Principles of Environmental Pollution. Blackie Academic andProfessional, London.Benaïssa, H. and Elouchdi, M.A. (2011).Biosorption of copper (II) ions from synthetic aqueous solutions by dryingbed activated sludge.Journal of Hazardous Materials194 69–78Fiol, N. et al., (2006) .Sorption of Pb(II), Ni(II), Cu(II) and Cd(II) from aqueous solution by olive stone waste, Sep,Purif,Technol.50 132–140.Fiol, N. et al., (2003). Biosorption of Cr(VI) using low cost sorbents, Environ. Chem. Lett. 1 135–139Hansen, H.K.., Arancibia, F., and Gutiérrez, C. (2010). Adsorption of copper onto agriculture wastematerials.Journal of Hazardous Materials 180 442–448He, Q. et al., (2007) . Biodegradability of tannin- containing wastewater from leather industry. Biodegradation, 18:465-472
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201331Ho, Y.S. and Mckay, G. (1999). Pseudo-second-order model for sorption processes. Process Biochemistry 34 451-465Ibrahim, M.N.M. ( 2010). A novel agricultural waste adsorbent for the removal of lead (II) ions from aqueoussolutions.Journal of Hazardous Materials,182 377–385Güngoğan, R.,Acemioğlu, B., & Alma, M.H.,(2004).Copper (II) adsorption from aqueous solution by herbaceouspeat.Journal of Colloids and Interface Science 269 303-309Johnson, M.A., (1997). Copper. In: Macrae, R. Robinson, R.K. and Sadler, M.J. (Ed.) Ency. Fd. Sci. Fd. Tech Nutri.Acad .Press, London. 1237- 1243.Kazemipour, M. et al., (2008). Removal of lead, cadmium, zinc, and copper from industrial waste water by carbondeveloped from walnut, hazelnut, almond, pistachio shell, and apricot stone. Journal of HazardousMaterials150 322-327.Khan, M.A. et al (2011).Biosorption and desorption of Nickel on oil cake: Batch and column studies. BioresourceTechnology.Khorramabadi, G.S. (2011).Utilisation of Immobilised Activated Sludge for the Biosorption of Chromium (VI).Can.J. Chem. Eng. 9999:1–8.Kosasih, A.N. (2011).Sequestering of Cu(II) from aqueous solution using cassava peel (Manihotesculenta).Journalof Hazardous Materials,180 366-374.Kumagai, S. (2010).”Molded micro-and mesoporos carbon/silca composite from rice husk and beet sugar”. ChemicalEng. Journal 156 270-277.Krishnani, K.K. (2008). Biosorption mechanism of nine different heavy metals onto biomatrix from ricehusk.Journal of Hazardous Materials153 1222-1234.Lagergren, S.(1898). About the theory of so-called adsorption of solublesubstances.KungligaSvenskaVetenskapsakademiensHandlingar 24, 1-6.Larous, S.,Meniai, A.H.,and Lehocine, M.B., (2005). Experimental study of the removal of copper from aqueoussolutions by adsorption using sawdust, Desalination 185 483–490.Li, Y.S., Liu, C.C.,and Chiou, C.S., (2004). Adsorption of Cr (II) from wastewater by wine processing waste sludge.Journal of Colloid Interface Science.273 95-101Lovett P.N., (2004). The shea butter value chain production, transformation and marketing in West Africa WathTechnical Report no. 2Naiya, T.K.,Chowdhury, P., Bhattacharya, A.K., Das,S.K. (2009).Sawdust and Neem bark as low-cost naturalbiosorbent for adsorptive removal of (II) ions from aqueous solutions. Chemical Engineering Journal14868–79.Nitiema, L.W. et al., (2010). Isolation of a Tannic Acid-Degrading Streptococcus sp.From an Anaerobic Shea CakeDigester.Pak. J. Biol. Sciences, 13: 46-50.Odukoya, O.O., and Ajayi, S.O., (1987). Trace heavy metals in Nigerian fishes II: Copper and Zinc. Nigerianjournal of Nutritional Sciences. Vol.8. pp 41-49.Oñate, C.E., (2009).Valorisation of Industrial waste for the removal of metals and Arsenic from aqueous effluents.Ph.D Thesis, University de Girona. ISBN: 978 84-692-3178-4 1-18Panda G.C.,Dasa, S.K., Bandopadhyay, T.S.,Guhaa, A.K., (2007). Adsorption of nickel on husk of Lathyrussativus:Behaviour and binding mechanism. Colloids and Surfaces B: Biointerfaces(57) 135–142.Villaescusa, I. et al., ( 2004). Removal of copper and nickel ions from aqueous solutions by grape stalks wastes,Water Res. 38 992–1002Wu, J.m Laird, D. A., Thompson. M.J., (1999). Sorption and Desorption of Copper on Soil Clay Components. J.Environ. Qual. 28: 334-338.Yahya, M.D. et al., (2012) .Equilibrium and Kinetic study on the removal of Lead from aqueous solution using Rawand Modified Shea Butter Cake .in: 42ndNigerian Society of Chemical Engineers Conference.Zhang, J. et al.,( 2011). Removal of Cu(II) from aqueous solution using the rice husk carbons prepared by thephysical activation process. Biomass and Bioenergy 35 464-472.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201332Table 1: Pseudo-1st–order for the removal of Cu (II) by MSBC at pH5 and 120 (mins)Ci (mgL-1) qe(exp.) (mgg-1) qe(calc.) (mgg-1) K1 (min-1) R2(linear) R2(non-linear)4 90.740 108.179 0.0152 0.5496 0.65846 137.315 90.386 0.0187 0.4333 0.649510 721.83 87.173 0.0119 0.581 0.7352Ci (mgL-1) qe(exp.) (mgg-1) qe(Calc.)(mgg-1) R2K2(gmg-1min-1) h (mgg-1min-1)4 89.8148 81.8148 0.9996 0.00100 8.10986 137.037 136.827 0.9999 0.00015 2.714610 229.629 230.032 1.0000 0.00002 1.122650 841.967 842.900 0.9895 0.00000 0.1012100 955.093 876.575 0.9753 0.00000 0.1933Table 2: Pseudo-2nd-order for the removal of Cu(II) by MSBC at pH 5 and Time 120(mins)
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201333Table 3: Langmuir and Freundlich parameters for Cu(II) sorption onto modified shea butter cake.Table 4: Comparison of amount adsorbed (qmax) of Cu(II) ions on other agricultural wastesAdsorbent Capacity (mg/g)Sorbent Langmuir Freundlich ReferenceRice Husk ash 2.30±0.2 28.8±0.02 Akhtar et al., 2010Rice husk biomatrix 10.9 6.21 Krishnani et al., 2008Herbaceous peat 4.84 8.86 Güdoĝan et al., 2004Rice husk carbons at 40oC 25.25 6.329 Zhang et al., 2011Modified shea butter cake 161.290 88.191 This workGrape Stalk 42.92 1.48 Onate, 2009Langmuir modelFreundlich modelCi(mg/L)qmax(mg/g)KL(L/g)RL ΔG0(kJ/mol)R2K(mg/g)1/n R24 564.972 4.425 0.0534 -3.709 0.9986 56.36 -0.0679 0.92286 86.207 57.999 0.0029 -10.128 0.9987 159.00 -0.0477 0.879410 161.290 310.000 0.0003 -14.308 1.0000 88.191 -0.0153 0.9668
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201335Fig. 3: SEM of Shea butter cake (RSBC) at (A) mag 1.00KX & (B) 3.00 KX
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201336Fig. 4: The percent removal of Cu(II) as a functionof time at various concentrations Fig.5: Percent removal of Cu(II) at different initial pHFig.6: Percentage removal and amount adsorbed of Cu (II) onmodified shea butter beads at varying adsorbent dosage00.050.10.150.20.250.380.082.084.086.088.090.092.00 50 100 150 200amountadsobed(mg/Bead)(%removal)Adsorbent dose (beads)% removal amount adsorbed (mg/bead)
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201337Fig.7: Pseudo-first–order kinetics of Cu(II) adsorption onto modified shea butter cake at 4mg/L and 6mg/LFig. 8 Pseudo-second-order Kinetics of Cu (II) adsorption onto modified shea butter cake at various initialconcentration
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201338Fig. 9: Langmuir adsorption isotherm at various initial Cu (II) concentrations 4; 6; 10mg/l on modifiedShea Butter CakeFig. 10: Freundlich adsorption isotherm at various initial Cu (II) concentrations 4; 6; 10mg/l on modifiedShea Butter Cake
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar